Max-Planck-Institut für Plasmaphysik, EURATOM Association Erosion and Deposition of Tungsten as Plasma-facing Material in ASDEX Upgrade. X. Gong 1 , K. Krieger 2 , J. Roth b , H. Maier 2 , V. Rohde 2 and ASDEX Upgrade Team 2
Max-Planck-Institut für Plasmaphysik, EURATOM Association
Erosion and Deposition of Tungsten as Plasma-facing Material in ASDEX Upgrade
X. Gong1, K. Krieger2, J. Rothb, H. Maier2, V. Rohde2 and ASDEX Upgrade Team2
1Institute of Plasma Physics, Academia Sinica, 230031 Hefei, Anhui, China 2Max-Planck-Institut für Plasmaphysik, IPP-EURATOM Association, 85748 Garching, Germany
The distribution of tungsten erosion along toroidal direction
Requirements for the next fusion device (ITER)
Tungsten as PFM at the central column of ASDEX Upgrade
The poloidal distribution of the tungsten erosion
Date evaluated by SIMNRA5.0 and WiNDF7.0
Summary of three experimental campaigns with tungsten as PMF in the ASDEX Upgrade
The spatial distribution of tungsten deposited on DivII and DivIIb
During plasma operation with tungsten as PFM, no negative influences on the plasma behaviour were observed, the tungsten concentration in the core plasma remaining below the maximum tolerable limit for fusion reactor relevant discharge scenarios 5,6.
During the present experiment, the W deposition is about two times larger than before, due to the additional source of tungsten from the midplane area, which is generally closest to the separatrix and used as ramp-down limiter.
Maximum W-deposition at inner divertor baffle module (nearby heat shield tiles),Similarly increased W-deposition at outer divertor,only small at the dome baffle.
The similar spatial distribution of deposited tungsten in both divertor configurations. A comparison of the total W-erosion with the deposition rates on the divertor shows that only 10% of the eroded tungsten deposited on the divertor, One can infer that most of the eroded tungsten migrates via direct transport channels in the outer scrape-off layer regions without penetrating the confined plasma. This is a good agreement with tungsten transport modelling by the DIVIMP code 10.
Ion Beam Analysis for W-coated tiles
1 G. Janeschitz, ITER JCT and HTs, J. Nucl. Mat. 290-293 (2001) 1-11
2 N. Peacock, et al., in: P. Stott, G. Gorini, E. Sindoni (Eds.), Diagnostics for experiment ThermonuclearFusion Reactors, Varenna, (Plenum, New York, 1996) p.291
3 K. Krieger, et al., ICFRM-10, 2001, submitted to J. Nucl. Mat.
4 A.Tabasso, H. Maier, K. Krieger, J. Roth, J. Nucl. Mat. 290-293 (2001) 326-330
5 R. Neu, et al., PPCF, 44 (2002) 811
6 V. Rohde, et al., 28th EPS, P1-042, 2001
7 K. Krieger, et al.,, PSI-15, O-14, 2002, submitted to J. Nucl. Mat.
 M.Mayer, Max-Planck-Institut für Plasmaphysik Report IPP 9/113 (1997)
9 N.P. Barradas, C.Jeynes, R.P.Webb, Appl. Phys. Lett. 71(1997) 291
10 A.Geier, et al., this conference
The tungsten coated graphite tiles were extended to the almost central column of ASDEX Upgrade in the present campaign 2002.Tungsten erosion and deposition were studied by ion beam analysis. Most of the W-coated tiles at the central column show both regions with net erosion and with local deposition. The maximum W-erosion rate was found to about 1.41014atom/cm2/s. The strong poloidal variation and the toroidal asymmetries of the tungsten erosion appears to correlate with the pattern of the scrape-off layer flux surfaces intersecting the surface of the inner column tiles. The maximum tungsten deposition was observed at the inner and outer divertor baffle modules, only small amounts of deposited tungsten were found at the divertor dome baffle. Comparison of the total W-erosion with the deposition rates in the divertor shows that only 10% of the eroded tungsten deposited in the divertor region.
Schematic of the W-coated tile showing the analysis points along poloidal and toroidal directions.
Red dots are RBS analyses of the W-coated tiles before plasma exposure. Average thickness of the original tungsten layer:
Thin tiles: 3.51017atoms/cm2 Thick tiles: 6.4 1018atoms/cm2
Analysis chamber with mainpulator for large W-coated tiles before and after experiment.
Ion Beam Analysis: RBS and PIXE using a 2.0MeV 4He ion beam and a 1.5MeV proton beam